Routine Quantitative Phase Analysis of Niobium-bearing Lateritic Ores
Post on 09-Dec-2016
Embed Size (px)
Routine quantitative phase analysis of niobium-bearing lateritic ores
Dona Kampata, Jean Naud and Philippe Sonnet
Universitk Catholique de Louvain Laboratoire de gkologie et mindralogie
3, Place Louis Pasteur I348 Louvain-la-Neuve, Belgium
Routine quantitative analyses by Rietveld full-pattern fitting have been carried out on more than one thousand niobium ore samples originating from four pyrochlore deposits: Lueshe and Bingo (D.R. Congo), Mabounie (Gabon), and Sokli (Finland). The ore samples were characterized by a highly variable mineral content, the presence of mineral phases with a wide range of compositions and a high amorphous content. An analytical procedure was established which addressed several problems: creation of an appropriate crystallographic parameter database, specimen preparation, check for preferred orientation and measurement of the amorphous content by the internal standard method.
X-ray powder diffraction combined with Rietveld full-pattern fitting is now widely accepted as a very promising technique for quantitative phase analysis. The technique, however, requires collecting a large set of input data: the crystal structure of all the different phases must be known, at least approximately, and several other parameters influencing the fit must be determined as well. This restriction makes the method particularly difficult to apply to mixtures involving a large number of phases when, in addition, each phase exhibits a variable chemical composition. This article describes the experience we have gained at analyzing such complex mixtures. Since 1991 on, we have analysed more than one thousand samples of niobium ore. These samples demonstrated considerable mineralogical variability. However, routine quantitative analysis was made possible by carefully defining and testing the analytical conditions. This research was performed as part of a group project performed by the London Natural History Museum (UK), the Ecole des Mines de Saint-Etienne (France) and the GfE Gesellschaft fur Elektrometallurgie mbH (Germany). It was partly funded by the European Commission within the framework of the BRITE-EURAM program.
Copyright(C)JCPDS-International Centre for Diffraction Data 2000, Advances in X-ray Analysis, Vol.42 379Copyright(C)JCPDS-International Centre for Diffraction Data 2000, Advances in X-ray Analysis, Vol.42 379ISSN 1097-0002
This document was presented at the Denver X-ray Conference (DXC) on Applications of X-ray Analysis. Sponsored by the International Centre for Diffraction Data (ICDD). This document is provided by ICDD in cooperation with the authors and presenters of the DXC for the express purpose of educating the scientific community. All copyrights for the document are retained by ICDD. Usage is restricted for the purposes of education and scientific research. DXC Website www.dxcicdd.com
ICDD Website - www.icdd.com
NIOBIUM ORE SAMPLES
The analyzed samples originate from four niobium deposits: Lueshe [ 1, 21 and Bingo  located in the Democratic Republic of Congo, Mabounie  in Gabon and Sokli [S, 61 in Finland (Figure 1). The deposits are found in rocks which can be qualified as carbonatite, a carbonate-rich rock of volcanic origin. The main niobium-bearing mineral in carbonatite is pyrochlore. In most carbonatite occurrences, the pyrochlore content in carbonatites is too low to be economically recovered. In the four deposits under review, economically mineable ore bodies (>1.5 wt. % NbzOs) formed where the carbonatite rock underwent weathering and dissolution. Pyrochlore, which is moderately resistant to weathering, accumulates in the residual soil formed by the dissolution of the carbonates close to the topographic surface. This process is most efficient in places where the soil was formed under lateritic conditions, i.e. in hot humid conditions similar to present day climates found in humid tropical regions of the world. The mineralogical composition of the ore is highly variable and complex. Four processes can be invoked to account for this variability. First, carbonatite bodies, even before weathering, are usually quite variable in composition, even at very small scale ( down to the centimetric scale). Second, lateritic weathering is a process which produces a pattern of successive layers with different mineral and chemical compositions that is called a weathering profile. In the deposits under investigation, between 3 to 5 zones formed down to a depth of 3 to 100 meters. Each zone is characterized by a definite mineral association or by the disappearance of a mineral which was present in the parent carbonatite rock. Third, weathering considerably modifies the chemical composition of the residual mineral, even if they resist dissolution. Fourth, weathering is a low temperature chemical process. It produces sluggish and incomplete mineral replacement reactions which eventually yield a high proportion of non-diffracting matter. These four processes explain to a large degree why the ore has a very variable mineral content. The variability makes it extremely difficult to devise an efficient ore treatment process. If the feed of the ore processing plant varies continuously, the setting of the plant must be continuously fine- tuned to keep pyrochlore losses at an acceptable level. One way to keep the feed constant is to blend the ores. In practice, one has to define several ore types and map where the different types occur within the deposit. Several ore blends must also be defined so that each blend corresponds to a particular setting of the plant. The analyses we performed aimed at defining such ore types and ore blends. Moreover, the analyses had to be performed within a time constraint of two weeks in order to provide a rapid response to on-going pilot plant tests.
Pyrochlore is currently the main economic mineral for niobium. Its formula is A2-xB206(0H,F)l _ .z H20. The mineral exhibits a large range of cation substitutions in the A- site: Ca, Na, K, Ba, B r, REE, U, Th, Mg, Mn, and Sn. The B-site essentially contains Nb but small amounts of Ti, Ta, Si and Zr can be found as well. Due to its high U and Th content (as in the Sokli deposit), pyrochlore is often metamict. In cases of high U and Th content, quantitative X-ray diffraction grossly underestimates the pyrochlore content. Therefore, for pyrochlore essaying, quantitative phase analysis must be complemented by chemical analyses.
Copyright(C)JCPDS-International Centre for Diffraction Data 2000, Advances in X-ray Analysis, Vol.42 380Copyright(C)JCPDS-International Centre for Diffraction Data 2000, Advances in X-ray Analysis, Vol.42 380ISSN 1097-0002
Figure 1 : Geographical position of the niobium ore deposits of Lueshe, Bingo, MabouniC and S6kli.
Copyright(C)JCPDS-International Centre for Diffraction Data 2000, Advances in X-ray Analysis, Vol.42 381Copyright(C)JCPDS-International Centre for Diffraction Data 2000, Advances in X-ray Analysis, Vol.42 381ISSN 1097-0002
Weathering not only increases the niobium content of the rock but it also considerably modifies the chemical composition of the residual pyrochlore. When occuring as weathered residual mineral, pyrochlore mineral is often strongly hydrated and exhibits a large A-cation deficiency [2, 6, 71. For example, the anhydrous Ca- and Na-rich pyrochlore present in unweathered rock is transformed into hydrated Ba-rich A-cation-depleted baryopyrochlore. Other residual minerals include amphiboles (several varieties often coexisted in the same sample), apatite, magnetite, ilmenite and a wide range of accessory minerals. Most of these minerals are also considerably modified by weathering. For instance, fluorapatite occuring initially transformed into carbonate-apatite (francolite). New minerals are created by the alteration of silicates: vermiculite, clay minerals, kaolinite, goethite, crandallite (calcium aluminophosphate). At each of the four deposit locations in our study, all these secondary minerals display highly variable composition. Finally, many of these minerals are imperfectly crystalized, some having only a weak diffraction power (crandallite at Sokli, for instance). In addition to having broader and weaker peaks, these minerals contribute to the non-diffracting part of the sample. For instance, comparing chemical analyses of the ore samples with their quantitative mineral compositions reveals that, in the Sokli deposit, crandallite represents a significant part of the amorphous fraction of the samples. As for the Lueshe deposit, goethite probably forms most of the amorphous fraction.
CRYSTAL STRUCTURE DATABASE
A database of crystallographic data for the various phases present in each deposit was established based on the available literature and existing crystal structure databases (ICDD-PDF, ICSD). This database includes minerals typically found in laterite (iron and aluminum oxides and hydroxides, phyllosilicates, . . . ) and mineral varieties that are specific to each of the deposits (apatite, aluminophosphate, carbonates, pyrochlore, amphiboles, . . .). One immediate question arises from the fact that the minerals in the ore sample do not have the same composition as the minerals in the database. Two methods were used to address this problem. The first method consists in: 1) collecting a range of several structure determinations and 2) choosing the structure model whose calculated diffraction pattern best fits the experimentally measured one. In many instances, the structure model which was chosen had a chemical composition which happened not to be the closest to the composition of the mineral in the sample. These chemical di